3-25-2019 Tool owner: Zuzanna Lewicka, [email protected]
609-258-1134, cell phone: 713-527-7194 Backup: Eric Mills,
, 609-258-4626, cell phone: 561-317-9872
Oxford PlasmaPro 100 PECVD Standard Operating Procedure
PROCEDURE OVERVIEW 1. Checking tool condition 2. Loading the wafer
3. Running deposition recipe 4. Running chamber cleaning
APPENDIX 1 – Aborting the Process APPENDIX 2 – Checking Process
CRITICAL PRECAUTIONS AND COMMON MISTAKES NEMO login controls the
monitor power MATERIALS restrictions:
• No exposed metal, photoresist, Kapton tape, or other organics;
Exceptions to this must be explicitly approved by the PRISM
SAMPLE restrictions: • All samples must be placed on a 4” wafer.
User must ensure that samples do not slide off of
carrier during loading (may require creation of custom holder)
• If loading/unloading by hand, put clean gloves immediately before
touching part to go inside the chamber
• If operating at a temperature higher than 70C, perform processing
afternoons/evenings only or reserve the tool at least two days in
Before you start: • Log into the tool using NEMO system • Check
wafer status in software, and visually (both chamber and loadlock)
• The loadlock should be pumped down, a wafer should be inside •
Oxford PC2000 (tool) Software should be running • The user “USER”
should be logged in
Tool condition for next user: • Ensure cleaning recipe has started,
wait for plasma to ignite and Logout • Clean up after yourself, do
not leave your items on the bench
1. Checking the tool condition
1.1 Reserve the tool using NEMO reservation system and select the
recipe that you planning to run.
1.2 Enable the tool in NEMO reservation system /Tool Control and
select the recipe that you planning to run.
1.3 If “Red Alert” is shown around the screen, stop and contact
cleanroom staff If “Yellow Alert” is shown around the screen, press
1.4 Check who is login to the system (USER or Manager). If it reads
anything other than “USER”, log in as user: Press System, then
Password, and enter USER/USER in the username/password boxes in the
1.5 Check if pumps are running. Go to Pumping page, from the System
menu and check that
turbo, backing, and roughing pump are all running (spinning
animation) and turbo is “at speed”. If Turbo pump is off, alert
PRISM cleanroom staff.
1.6 Check chamber vacuum (Penning <~3e-07 Torr) 1.7 Check that
no wafer is shown in the process chamber, and that there is a wafer
in the loadlock. Also, visually check that the wafer has been
unloaded into the loadlock.
2. Loading the wafer
2.1 Visually check that the wafer has been unloaded into the
loadlock 2.2 Vent the loadlock. Under the loadlock interface, click
Stop. For popup, “Wafer … has
finished processing” click OK. Then, under the loadlock interface,
click Vent. 2.3 Wait until “Vent Time Left” countdown reaches 0.
This will take 4 minutes.
2.4 Open the loadlock by pulling upwards on the black knob on the
loadlock door (no twisting). 2.5 Gently place 4” wafer on the
loadlock tray, up against the round cams (circled), with the
flat facing towards the process chamber. Make sure the edge of your
sample lines up with marker line.
NOTE: Put on clean gloves before handling wafer.
2.6 Close the loadlock door and Click “Stop”, then “Evacuate” under
the loadlock interface. 2.7 In the popup, enter a sample name and
press “OK” to indicate a wafer in the loadlock. 2.8 When "Cycling
Loadlock Pumping" is displayed under the loadlock interface, the
good enough for your recipe to be run.
3. Running deposition recipe
NOTE: For reproducible results, before deposition on a real sample,
it is recommended to condition the clean chamber by depositing >
100 nm of SiO2
or SiN film on conditioning wafer.
3.1 To load the desired deposition recipe, click Process Menu, then
Recipes. 3.2 Select desired recipe and click Load. 3.3 For a popup
reading: “Currently loaded recipe contains unsaved changes. …..”
This will restore the recipe to the staff programmed defaults. 3.4
Find your desired recipe from the pop-up list and click OK.
NOTE: If heating the chamber from 70 C to 250 C, run the “@Heat
Chamber to 250C” process before running your conditioning and
deposition processes. This
will take ~25 minutes.
3.5 To adjust deposition time, left-click on the “Dep” step in the
recipe, then click “Edit Step” NOTE: click on the step in the white
box of the Recipe Editor window, not the step library.
3.6 Change the step time (circled) to deposit desired thickness of
material. NOTE: you can only change step time, not other
parameters. 3.7 Click “OK” to exit the editing screen.
3.8 From Recipes page, click “Run”, will hear pump whirring get
louder. NOTE: sample will be loaded from loadlock into chamber
automatically and process page will come up automatically.
3.9 Monitor deposition process. Wait through “Pump”, “Purge” and/or
“Preheat” steps. 3.10 Once “Dep” step begins, watch if RF power
stabilize on screen. If Reflected Power (red
squares in the picture) does not stabilize at < 5W, contact the
PRISM Cleanroom staff.
3.11 Watch for plasma to ignite and stabilize in chamber. If plasma
is not visible once RF power has stabilized, abort the process and
inform the staff.
3.12 Once process is complete, a “Yellow Alert” pop-up will appear.
Click “Continue” and wait ~30s for wafer unload sequence to
4. Running chamber cleaning recipe
4.1. Load cleaning recipe by clicking Process Menu, then Recipes
then Load, and choose appropriate cleaning recipe:
i) “Chamber Clean @70C” if you deposited at 70C ii) “Chamber Clean
@250C” if you operated at 250C
3.13 Adjust cleaning time in both steps: high pressure clean-auto
and low pressure clean-
auto by editing the step time in Process Step Editor. Note: To etch
back 1um of deposited material: the “high pressure clean” step must
run for 12 minutes, and the “low pressure clean” step must run for
9 minutes. A high pressure and a low- pressure CF4/N2O steps are
designed to chemically etch the deposited SiO2/SiNx:
• The high-pressure step is designed to remove the bulk of the
deposited material, using a relatively low ion-bombardment
• The low-pressure step is designed to remove any remaining
deposited material, using a high ion-bobardment strength
In the cleaning recipe, there is also a set of 50 pump/purge cycles
after these plasma steps, designed to induce flaking of any thick
material that was only partially-attacked during the plasma
3.14 Press the “Run” button and run the cleaning recipe. 3.15 Wait
for the plasma to ignite and stabilize before leaving the tool.
This should happen
after about 1 minute.
3.16 Sign out of the tool in NEMO NOTE: Fill Logbook page in NEMO:
Recipe and Approximate Film Thickness; If you running chamber
cleaning recipe, “prevent others from using the tool for 60
APPENDIX 1 – Aborting the process 1. To abort a process, click the
STOP button, on the process page.
NOTE: If you stop a process, or it aborts due to a hardware fault,
a dialog box will pop up asking if you want your sample moved to
the loadlock. Always click yes!!! If you click no, the staff will
have to assist you to unload your sample manually. A
successfully-aborted process will result in your wafer being
returned to the loadlock, where you’ll see the “Yellow alert”, and
a “Process Failed” popup. Remove your wafer, and contact the MNFL
APPENDIX 2 - Checking Process Logs 1. To check Process Logs: Click
Process, then Log View. 2. In the Log Viewer screen find your
process. NOTE: It is easier to find your process if you first,
uncheck the “Process Step” box under “Filter by Type”. Next, select
your desired date range (2-3 weeks is usually enough to find the
recipe of interest). 3. Left-Click on the process of interest, then
left-click “View Run” (top-right corner)
4. Now you’re viewing all of the sensor readings taken during the
particular step of the
process. Time is displayed as a countdown, in seconds. Scroll right
to see further into each process step.
5. You can move forward/backwards by step, clicking the “Prev” and
“Next” buttons (right side of screen), and see the current step
name under “Recipe Step Details” (top of the screen)